3D Printing of Transparent GlassSusanne Klein, Steve Simske, Carinna Parraman, Peter Walters, David Huson, Stephen HoskinsHP LaboratoriesHPL-2012-198Abstract:Traditional assembly line manufacturing is speculative, costly and environmentally unsustainable. It isspeculative because it commits substantial resources—energy, materials, shipping, handling, stocking anddisplaying—without a guaranteed sale. It is costly because each of these resources—material, process,people and place—involves expense not encountered when a product is manufactured at the time of sale.It is environmentally unsustainable because, no matter how much recycling is done, not using theresources unless actually needed is always a better path.As part of the RAGNAROK (Research on Advancing Glass & Nonorganic Applications to RecreateObjects & Kinetics) project in HP Labs, we identified glass as a promising candidate for additivemanufacturing based on 3-D printing methods. Glass is a silica-based material. With 90% of the earth’scrust composed of silicate minerals, there will be no shortage of silica resources. Glass is easy to recycleand is environmentally friendly. Glass is inexpensive but looks precious, is pleasant to the touch and is sofamiliar that customers will not be disappointed by its fragility— under certain conditions.A major need, and concomitantly a major challenge, for 3D printed glass is transparency. We will discussseveral methods how to achieve it.External Posting Date: September 6, 2012 [Fulltext] Approved for External PublicationInternal Posting Date: September 6, 2012 [Fulltext] Copyright 2012 Hewlett-Packard Development Company, L.P.
3D Printing of transparent glass 1 2 1 3 3 3 3 1Susanne Klein , Steve Simske , Guy Adams , Carinna Parraman , Peter Walters , David Huson , Stephen Hoskins ; HP Labs, Bristol 2 3UK; HP Labs, Fort Collins, USA; Centre for Fine Print Research, Bristol, UK a solution of for example sodium silicate or liquid glassAbstract shows reduced scattering. But pastes made like that are not Traditional assembly line manufacturing is speculative, costly printable. Under pressure, the solution is squeezed out of theand environmentally unsustainable. It is speculative because it paste and jamming occurs. This is a well-known phenomenoncommits substantial resources—energy, materials, shipping, easily observed when walking on wet sand on the beach.handling, stocking and displaying—without a guaranteed sale. It is Firing causes gas formation even with well dried green warecostly because each of these resources—material, process, people which leads to bubbling of the sample and loss of all detail asand place—involves expense not encountered when a product is shown in figure 1.manufactured at the time of sale. It is environmentallyunsustainable because, no matter how much recycling is done, notusing the resources unless actually needed is always a better path. As part of the RAGNAROK (Research on Advancing Glass &Nonorganic Applications to Recreate Objects & Kinetics) projectin HP Labs, we identified glass as a promising candidate foradditive manufacturing based on 3-D printing methods. Glass is asilica-based material. With 90% of the earth’s crust composed ofsilicate minerals, there will be no shortage of silica resources.Glass is easy to recycle and is environmentally friendly. Glass isinexpensive but looks precious, is pleasant to the touch and is so Figure1: Glass sample with sodium silicate solution as the index matchingfamiliar that customers will not be disappointed by its fragility— fluid. Firing of the sample leads to bubbling and loss of all detail.under certain conditions. A major need, and concomitantly a major challenge, for 3Dprinted glass is transparency. We will discuss several methods howto achieve it. Big glass grains3D Printing and warm glass Scattering has only little influence on the transmitted light Warm glass or kiln glass is the oldest glass manufacturing when the diameter of the scatterer is either bigger than ~ 20 method. Glass powder, or frit, is shaped in a mold and fired at µm or smaller than 400 nm, independent of the refractive moderate temperatures. The powder fuses and a solid glass index difference between scatterer and surrounding medium object is the result. Depending on firing temperature and (see for example ). We have found that glass frit with duration, the glass grains just stick and keep their sandy particle sizes between 38 µm and 75 µm results in transparent appearance or melt together and form a smooth body. The samples with major difference between kiln glass and blown glass is that the molten glass mass is not agitated in the kiln glass process. Therefore kiln glass contains many more air bubbles than blown glass. This has consequences for the transparency of the final glass object. The finer the frit, the better the detail but the more prevalently that the air bubbles are trapped. This scatters the transmitted light and turns the object opaque. 3D printing cannot replace the firing process, but does make the mold obsolete. The key to transparency is the ‘ink’. We will concentrate on extrusion printing, but the same principals apply to powder bed printing. Figure 2: Transparent glass sample with air inclusions. There are three ways to suppress scattering and reach transparency: a) index matching between glass grain and solvent, b) big glass grains, and c) small glass grains. sufficient detail. In figure 2 air inclusions are clearly visible.Index match Note the choice of binder can have a negative effect on Glass grains become invisible -- that is, non-scattering – transparency as well. We followed first the recipes published when the solvent they are suspended in has the same by the University of Washington  and added approximately refractive index as the glass. Indeed, a suspension of glass in
40wt% of polysaccharides to the glass water mixture. order of a micron in size, which leads to the opaque Polysaccharides caramelize at temperatures between 110ºC appearance. This assumption will be further investigated. and 180º. Above 250⁰C caramel decomposes into carbon mon- and di-oxide, hydrocarbons, alcohols, aldehydes, ketones and several furan derivatives which are volatile . If the caramel is trapped inside the sample, this decomposition is incomplete and leads to a discolouration of the sample (see figure 3). The polysaccharide content has to be reduced drastically to avoid this effect.Figure 3: For glass sample on the left 40wt% of saccharides were used asbinder, for the one on the right only 5wt%. The left on is discoloured, the right Figure 5: On the left, the sample is made from particles with an averageone not. diameter of 700 nm. On the right, the average particle size was 50 µm. Both samples were fired following the same firing schedule.Small glass grains As mentioned before scattering should be negligible for 3D Printing and Cold glass particles smaller than 400nm (spherical) diameter. Glass is a Cold glass stands for all materials where glass is used in a brittle material. Milling leads quickly to sub-micron particle strengthening component in another cured matrix. The weight sizes. In figure 4 a typical number size distribution is shown. percentage of the glass component is only between 5 and 20 Even though the average particle size is about 700 nm the wt% and curing does not rely on fusing of the glass particle. majority of particles are below 400 nm diameter. First experiments show that the toughness and elasticity of natural polymers change with the amount of added glass frit. A low weight percentage of glass reduces shrinkage but the mechanical characteristics of the sample after drying are governed by those of the polymer. The sample becomes tougher but more brittle with increasing glass content. Beyond 50wt% of glass we find a decline in elastic strength. The elasticity of the polymer makes it possible to apply the glass polymer film on elastic substrates. The best results achieved so far are with materials with are index matched to the glass particles. Index matching helps particle dispersion and suppresses scattering independent of particle size.Figure 4: Typical number distribution of a milled glass sample. Please notethat the x-axis is the radius and not the particle diameter. All milled glass samples show excellent detail but are opaque and have an appearance more like ceramic than vitreous appearance. Why? Density measurements show that sub-micron particles have a random packing after firing, whereas particles with diameters in the micron range have a density so high that the single particles must have melted and flowed together. This result is counterintuitive and demands further investigation. Random packing means that the sample has only ~ 60% of the density of a solid block of glass; the rest is trapped gas. These gas Figure 6: Micrograph of a translucent polymer string with 60wt% glass pockets are scatterers in their own right and probably on the loading. Glass index and polymer index are matched. The glass particles are not visible but scattering is caused by air inclusions clearly visible as round and elongated bubbles.
References Author Biography H.C. van de Hulst, Light scattering by small particles (Courier Dover Susanne Klein holds a Diploma in Physics and a PhD in Medical publications, 1957) Physics from the University of Saarland. Since 1995 she has worked and http://www.washington.edu/news/archive/id/52160 lived in the UK, first as a Royal Society Research Assistant at the P. Tomasik, “The thermal decomposition of carbohydrates. Part I. The University of Bristol and then as a member of HP Labs. Her main research decomposition of mono-, di-, and oligo-saccharides,” Advances in interests lie in new materials for displays and 3D printing. Carbohydrate Chemistry and Biochemistry, 47, 203 (1989).